A Family of Porous Lonsdaleite-e Networks Obtained through Pillaring of Decorated Kagomé Lattice Sheets
Alexander Schoedel; Wesley Boyette; Lukasz Wojtas; Mohamed Eddaoudi; Michael J. Zaworotko; Journal of the American Chemical Society 135 (2013) 14016–14019; doi:10.1021/ja406030p

data_4120832
_publ_section_title
;
 A Family of Porous Lonsdaleite-e Networks Obtained through Pillaring of
 Decorated Kagom\'e Lattice Sheets
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              14016
_journal_page_last               14019
_journal_paper_doi               10.1021/ja406030p
_journal_volume                  135
_journal_year                    2013
_chemical_formula_sum            'C86 H48 Cr3 N6 O42 Zn6'
_chemical_formula_weight         2385.52
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           194
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   18.9479(4)
_cell_length_b                   18.9479(4)
_cell_length_c                   35.9127(8)
_cell_measurement_temperature    100(2)
_cell_volume                     11166.1(4)
_computing_cell_refinement       'APEX2 (Bruker, 2010); SAINT (Bruker, 2009)'
_computing_data_collection       'APEX2 (Bruker, 2010)'
_computing_data_reduction        'SAINT (Bruker, 2009);XPREP(Sheldrick,2008)'
_computing_publication_material  'APEX2 (Bruker, 2010)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      100(2)
_diffrn_measured_fraction_theta_full 0.991
_diffrn_measured_fraction_theta_max 0.991
_diffrn_measurement_device_type  'Bruker D8 Venture PHOTON 100 CMOS'
_diffrn_measurement_method       'omega scans'
_diffrn_radiation_monochromator  mirrors
_diffrn_radiation_source         'INCOATEC Imus micro-focus source'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.0467
_diffrn_reflns_av_sigmaI/netI    0.0224
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       -22
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_l_max       42
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            44353
_diffrn_reflns_theta_full        69.03
_diffrn_reflns_theta_max         69.03
_diffrn_reflns_theta_min         2.46
_exptl_absorpt_coefficient_mu    2.207
_exptl_absorpt_correction_T_max  0.8977
_exptl_absorpt_correction_T_min  0.8095
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS; (Sheldrick, 2003)'
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    0.710
_exptl_crystal_description       plate
_exptl_crystal_F_000             2388
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.05
_refine_diff_density_max         0.744
_refine_diff_density_min         -0.460
_refine_diff_density_rms         0.050
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.073
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     125
_refine_ls_number_reflns         3837
_refine_ls_number_restraints     6
_refine_ls_restrained_S_all      1.084
_refine_ls_R_factor_all          0.0655
_refine_ls_R_factor_gt           0.0513
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.1103P)^2^+1.2733P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1701
_refine_ls_wR_factor_ref         0.1792
_reflns_number_gt                2829
_reflns_number_total             3837
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja406030p_si_004.cif
_cod_data_source_block           tp-PMBB-1-lon-e-H
_cod_database_code               4120832